Inorg. Chem. 2009, 48, 3145-3152
Synthesis, Structural Characterization, and Electronic Structure of
Single-Crystalline CuxV2O5 Nanowires
Christopher J. Patridge,† Cherno Jaye,‡ Hengsong Zhang,† Amy C. Marschilok,§ Daniel A. Fischer,‡
Esther S. Takeuchi,†,§,| and Sarbajit Banerjee*,†
Department of Chemistry, Department of Electrical Engineering, and Department of Chemical and
Biological Engineering, UniVersity at Buffalo, State UniVersity of New York, Buffalo,
New York 14260-3000, and Materials Science and Engineering Laboratory, National Institute of
Standards and Technology, Gaithersburg, Maryland 20899
Received December 17, 2008
Single-crystalline copper vanadium oxide nanowires ′-CuxV2O5 (x ∼ 0.60) have been synthesized by the
hydrothermal reduction of bulk CuV2O6 using small-molecule aliphatic alcohols as reducing agents. The prepared
copper vanadium bronze nanowires are metallic in nature and exhibit aspect ratios as high as 300. The recent
discovery of superconductivity and charge disproportionation in bulk ′-CuxV2O5 has led to renewed interest in
these one-dimensional metallic systems. Scaling these systems to nanoscale dimensions offers the potential for
further tunability of electronic transport and Li-ion intercalation kinetics. A combination of spectroscopic and electrical
measurement methods has been used to provide evidence for the metallic nature and the presence of room-
temperature charge disproportionation in these nanowires.
Introduction tions,3 charge and spin ordering,4 paramagnetism,5 gapless
states, and superconductivity.5 The facile variations in
The incorporation of monovalent and divalent metals into
stoichiometry that can be achieved in these systems6-10 point
the layered framework of vanadium pentoxide has been
to the possibility of ﬁnely tuning electron transport in these
studied extensively over the last ﬁfty years. The wide range
materials. Wadsley et al.11 reported the ﬁrst vanadium
of available oxidation states of vanadium provides a myriad
bronzes incorporating Na+ ions with the stoichiometry
of compounds and coordination modes. Of the different
NaxV2O5 and showed that the addition of metal cations does
stoichiometric vanadium oxides, the tunnel-like framework
not signiﬁcantly alter the structure and size of the V2O5
of V2O5 is especially notable since it allows the facile
framework. The V2O5 tunnel framework is composed of three
intercalation of a variety of organic and inorganic guest
crystallographically distinct vanadium sites. The ﬁrst set of
species.1,2 A rich diversity of vanadium bronzes and inter-
vanadium atoms (V1) lie at the centers of VO6 octahedra
calation compounds based on the incorporation of either
alkali or transition metals within the interstitial spaces of
(3) Villeneuve, G.; Kessler, H.; Chaminade, J. P. J. Phys., Colloq. 1976,
the V2O5 tunnel framework have been extensively studied (4), 79–82.
in recent years. Vanadium bronzes show very remarkable (4) Yamaura, J.; Yamauchi, T.; Ninomiya, E.; Sawa, H.; Isobe, M.;
Yamada, H.; Ueda, Y. J. Magn. Magn. Mater. 2004, 272-276 (1),
transport and magnetic properties some of which have only 438–439.
recently been discovered including metal-insulator transi- (5) Ueda, Y.; Isobe, M.; Yamauchi, T. J. Phys. Chem. Solids 2002, 63
(6) Gopalakrishnan, R.; Chowdari, B. V. R.; Tan, K. L. Solid State Ionics
* To whom correspondence should be addressed. E-mail: sb244@ 1992, 53-56 (2), 1168–71.
buffalo.edu. (7) Kato, K.; Takayama-Muromachi, E.; Kanke, Y. Acta Crystallogr., Sec.
Department of Chemistry, State University of New York, Buffalo. C 1989, C45 (12), 1845–1847.
National Institute of Standards and Technology. (8) Kato, K.; Takayama-Muromachi, E.; Kanke, Y. Acta Crystallogr., Sec.
Department of Electrical Engineering, State University of New York, C 1989, C45 (12), 1841–1844.
Buffalo. (9) Nagao, N.; Nogami, Y.; Oshima, K.; Yamada, H.; Ueda, Y. Phys. B:
Department of Chemical and Biological Engineering, State University Cond. Mat. 2003, 329-333 (2), 713–714.
of New York, Buffalo. (10) Pereira-Ramos, J. P.; Messina, R.; Znaidi, L.; Bafﬁer, N. Solid State
(1) Livage, J. Chem. Mater. 1991, 3 (4), 578–593. Ionics 1988, 28-30 (1), 886–894.
(2) Wang, Y.; Cao, G. Z. Chem. Mater. 2006, 18 (12), 2787–2804. (11) Wadsley, A. D. Acta Crystallogr. 1955, 8, 695–701.
10.1021/ic802408c CCC: $40.75 2009 American Chemical Society Inorganic Chemistry, Vol. 48, No. 7, 2009 3145
Published on Web 03/04/2009
Patridge et al.
that share edges to form double chains; the second set of anisotropy between excellent conduction along the b-axis and
vanadium atoms (V2) lie at the centers of VO6 octahedra poor conduction along the a and c axes. Indeed, Ma et al.
that form two-legged ladder-like layers by sharing corners; have proposed that the superconductivity observed at high
the third set of vanadium (V3) sites are within VO5 square pressures originates from charge transfer from partially
pyramids that share edges to form double chains. The zigzag occupied V1-V3 chains to V2-V2 ladders.15a The avail-
double-chain and ladder-like framework formed by the VO6 ability of highly anisotropic 1D nanowires with lateral
and VO5 polyhedra along the b-axis constitute a tunnel dimensions smaller than the coherence length will allow the
structure that is able to accommodate cations at speciﬁc sites. investigation of quantum phase slip properties that give rise
Two distinct classes of MxV2O5 bronzes are known ( and to ﬁnite resistance below Tc in these novel super-
′) that essentially retain the V2O5 tunnel framework and conductors.15b The Mermin-Wagner theorem states that
differ only in the sites occupied by the metal cations. Most long-range superconducting order can not exist in a truly
cations upon incorporation into the V2O5 framework yield 1D system; the fabrication of single-crystalline vanadium
-MxV2O5 bronzes wherein they occupy a 5-coordinated site bronze nanowires will enable evaluation of the role of
within the tunnels; in the -phase the chains of cations are thermal and quantum phase slips in broadening and extin-
separated by 2.2-2.3 Å, and owing to this small separation, guishing superconductivity in these materials. The extent of
nearest neighbor sites in the ac plane can not be simulta- copper doping also strongly inﬂuences the magnetic
neously occupied, yielding a theoretical maximum value of susceptibility,15a structural charge ordering,12,4 and bipolaron
x ) 0.33.12 In contrast, Li+ and Cu+ yield ′-MxV2O5 bronzes formation16,17 in CuxV2O5.18
wherein metal ions occupy tetrahedral MO4 and trigonally More recently, the high conductivity and increased inter-
coordinated MO3 sites that are shifted by half a unit cell layer separation in copper vanadium bronzes has led to their
length from the sites occupied in the phase. The separation exploration as high-capacity cathode materials for Li-ion
between chains of cations that are thus coordinated is batteries.19-23 Scaling copper vanadium bronzes to nanoscale
signiﬁcantly larger than for the phase, approaching close dimensions offers the opportunity to further tune electronic
to 3.7 Å.12 The smaller size and greater separation between transport, magnetic properties, and the Li-ion storage capaci-
cations allows the incorporation of signiﬁcantly greater ties and intercalation kinetics of these systems. In terms of
amounts of Cu ranging up to a theoretical maximum of x ) their use as cathode materials, nanostructured copper vana-
0.67.13 In a series of articles, the groups of Ueda, Yamaura, dium bronzes may potentially show improved power and
and Yamada have painstakingly mapped out the phase energy densities because of improved solid-state diffusion
diagram of CuxV2O5 as a function of temperature, pressure, kinetics, better interfacial contact with the electrolyte, and
and Cu concentration.5,9,12,14 The ground-state of the ′ phase the operation of Li-ion storage mechanisms not accessible
is characterized by metallic behavior for x > 0.40. Indeed, for bulk materials.24 Recently, Cui and co-workers have
the conductivity of the ′-copper vanadium bronzes shows demonstrated the completely reversible lithiation and delithi-
a signiﬁcantly decreased transport barrier as the Cu content ation of high-aspect-ratio sub-100 nm diameter V2O5 nanow-
increases to ∼0.60.12 However, unlike -MxV2O5 phases that ires even for lithiated phases LixV2O5 with x approaching
show discontinuous insulator-metal phase transitions with 3.0.25 In contrast, in bulk V2O5 the lithiation process (and
the increasing incorporation of metal ions, the CuxV2O5 ′- the formation of the lithium vanadium bronze) is irreversible
phases tend to show a smooth increase in conductivity with at such stoichiometries. The greater conductivity of the
increasing copper concentration. The conductivity of both CuxV2O5 nanowires compared to V2O5 (an n-type semicon-
and ′ phases arises from the reduction of V5+ framework ductor) is likely to lead to improved Li-ion insertion/
ions to V4+ followed by one-dimensional (1D) charge extraction kinetics and better cycling behavior. A longstand-
ordering along the framework. Several possible charge ing objective in the electrochemistry community has been
ordering patterns have been proposed to explain conduction the fabrication of novel battery architectures based on arrays
through the tunnel framework including a linear chain or of nanowires/nanorods vertically aligned on collector elec-
rectangular charge ordering pattern on the V2-V2 ladder trodes such that the charging/discharging of individual
for various -M0.33V2O5 bronzes and a straight-chain charge (16) Chakraverty, B. K.; Sienko, M. J.; Bonnerot, J. Phys. ReV. B 1978,
disproportionation motif accompanied by structural deforma- 17 (10), 3781.
tion on the V2-V2 ladder for ′-Cu0.65V2O5.15a Indeed, (17) Nagasawa, H.; Onoda, M.; Kanai, Y.; Kagoshima, S. Synth. Met. 1987,
19 (1-3), 971–976.
superconductivity has been observed at around 3 GPa (18) Nithya, R.; Chandra, S.; Reddy, G. L. N.; Sahu, H. K.; Sastry, V. S.
pressure and 6 K for the ′-Cu0.65V2O5 phase.5 The crystal Los Alamos Natl. Lab. Cond. Mater. 2004, 1–9.
(19) Andrukaitis, E. J. Power Sources 1997, 68 (2), 652–655.
structure of the superconducting phase is characterized as a (20) Andrukaitis, E.; Cooper, J. P.; Smit, J. H. J. Power Sources 1995, 54
quasi 1D system at high pressure because of the large (2), 465–469.
(21) Li, H. X.; Jiao, L. F.; Yuan, H. T.; Zhao, M.; Zhang, M.; Wang, Y. M.
(12) Yamada, H.; Ueda, Y. J. Phys. Soc. Jpn. 2000, 69 (5), 1437–1442. Mater. Lett. 2007, 61 (1), 101–104.
(13) Streltsov, V. A.; Nakashima, P. N. H.; Sobolev, A. N.; Ozerov, R. P. (22) Souza, E. A.; Lourenco, A.; Gorenstein, A. Solid State Ionics 2007,
Acta Crystallogr., Sec. B 2005, B61 (1), 17–24. 178 (5-6), 381–385.
(14) Yamaura, J.-I.; Yamauchi, T.; Isobe, M.; Yamada, H.; Ueda, Y. J. (23) Wei, Y.; Ryu, C.-W.; Kim, K.-B. J. Power Sources 2007, 165 (1),
Phys. Soc. Jpn. 2004, 73 (4), 914–920. 386–392.
(15) (a) Ma, C.; Yang, H. X.; Li, Z. A.; Ueda, Y.; Li, J. Q. Solid State (24) Arico, A. S.; Bruce, P.; Scrosati, B.; Tarascon, J.-M.; van Schalkwijk,
Commun. 2008, 146 (1-2), 30–34. (b) Lau, C. N.; Markovic, N.; W. Nat. Mater. 2005, 4 (5), 366–377.
Bockrath, M.; Bezryadin, A.; Tinkham, M. Phys. ReV. Lett. 2001, 87, (25) Chan, C. K.; Peng, H.; Twesten, R. D.; Jarausch, K.; Zhang, X. F.;
217003/1–217003/4. Cui, Y. Nano Letters 2007, 7 (2), 490–495.
3146 Inorganic Chemistry, Vol. 48, No. 7, 2009
Single-Crystalline CuxV2O5 Nanowires
nanowires controls the power rate of the battery. The highly instrument (Cu KR radiation, voltage 40 kV, current 44 mA). The
anisotropic CuxV2O5 nanowires prepared here are likely to samples were ground to a ﬁne powder and packed in a sample
be excellent building blocks for such cathode geometries. holder with 0.5 mm depth for the powder XRD measurements.
The small lateral dimensions of these nanowires are condu- Pattern ﬁtting and phase identiﬁcation were achieved with the help
of JADE 8.5. The morphology of the hydrothermally prepared
cive to rapid Li-ion insertion, extraction, and diffusion,
product was evaluated by scanning electron microscopy (Hitachi
whereas the long lengths will provide high storage capacities.
S4000 cold ﬁeld emission at 25 kV), transmission electron
In this Article, we report the ﬁrst synthesis of single- microscopy (JEOL-100-CX-II at 100 kV operating voltage), and
crystalline metallic copper vanadate nanowires with aspect by combining high-resolution transmission electron microscopy
ratios exceeding 300. The availability of these novel 1D (HRTEM) with selected area electron diffraction (SAED, JEOL-
nanostructures will provide new insight into the effect of 2010, 200 kV, 100 µA). For electron microscopy observations, the
ﬁnite size on electron transport and Li-ion intercalation in samples were dispersed in 2-propanol using a bath sonicator and
copper vanadium bronzes. A previous report in the literature then deposited onto 300 mesh carbon-coated Cu grids. High-
points to the fabrication of CuV2O6 nanowires via the resolution X-ray photoelectron spectroscopy (XPS) data was
hydrothermal reaction of aqueous NH4VO3 and CuCl2.26 obtained using a Perkin-Elmer PHI 660 instrument. Four-point
However, the absence of V4+ makes this system less probe electrical measurements of CuxV2O5 nanowire pellets were
made using a home-built apparatus based on a Keithley-220 current
interesting from both solid-state physics and electrochemical
source and a Keithley-6517 power supply. Fourier transform
perspectives since the primary conduction path is thought
infrared (FTIR) data was obtained on a Nicolet Magna 550
to be along V4+ ladders. Furthermore, the R-CuV2O6 nanow- instrument in transmission mode for pellets prepared by mixing
ires synthesized via the hydrothermal approach are poly- the samples with KBr. Near-edge X-ray absorption ﬁne structure
crystalline with a very high density of grain boundaries. (NEXAFS) spectroscopy data was collected on National Institute
Slightly oxygen-deﬁcient hydrated MxV2O5-xH2O nanowires of Standards and Technology beamline U7A at the National
have also been previously reported in the literature but the Synchrotron Light Source of Brookhaven National Laboratory with
hydrated structure shows signiﬁcant differences from that a toroidal mirror spherical grating monochromator using a 1200
of vanadium bronzes.27 Furthermore, Liu et al. have reported lines/mm grating and an energy resolution of 0.1 eV. NEXAFS
the fabrication of single-crystalline Ag0.33V2O5 nanowires by spectra were collected in partial electron yield (PEY) mode with a
the hydrothermal reaction of aqueous AgNO3 with channeltron multiplier near the sample surface using the detector
at -200 V bias to enhance surface sensitivity. The PEY signal was
NH4VO3.28 Most notably, Balkus and co-workers have
normalized by the drain current of a clean gold mesh located along
reported the clean synthesis of ultralong orthorhombic V2O5
the path of the incident X-rays. In addition, all the data was collected
nanowires and have also extended this synthesis to the in conjunction with a standard V reference mesh for energy
preparation of silver vanadium oxide structures.29 Here, we calibration.
use the hydrothermal reduction of a solid-state CuV2O6
precursor by small-molecule aliphatic alcohols to form Results and Discussion
single-crystalline Cu0.60V2O5 nanowires with high aspect The bulk CuV2O6 precursor prepared by the high-temper-
ratios. ature solid-state reaction has been characterized by XRD.
Experimental Section The XRD reﬂections can be indexed to a triclinic phase of
CuV2O6 (Joint Committee on Powder Diffraction Standards
Synthesis. Bulk CuV2O6 powder was synthesized by mixing CuO
powder (Sigma-Aldrich >99%) and V2O5 powder (Sigma-Aldrich
(JCDPS) 00-045-1054, a ) 9.172 Å, b ) 3.546 Å, c ) 6.482
99.5%) in 1:1 molar ratio.30,31 The mixture was heated in a mufﬂe Å; R ) 92.3, ) 110.32, γ ) 91.85). After hydrothermal
furnace at 620 °C for 48 h and then allowed to cool to room reduction with aliphatic alcohols, XRD data indicates that
temperature. Next, 300 mg of the prepared CuV2O6 product was CuV2O6 is converted to CuxV2O5 with x estimated to be
placed in a Teﬂon cup and heated in a sealed autoclave (Parr) along 0.55-0.65. The product diffraction pattern can be indexed
with 0.1-4.0 mL of 2-propanol mixed with deionized water to bring to a monoclinic phase of Cu (0.55 - 0.65)V2O5 (JCDPS 79-007-
the total liquid volume to 16 mL. The hydrothermal reaction was 7609) with a ) 15.2007 Å, b ) 3.6725 Å, c ) 10.0927 Å,
performed for 3-7 days at 210 °C. Upon cooling to room ) 106.31°18,32,33 along with some other minor phases as
temperature, the solid product was vacuum-ﬁltered, washed repeat- discussed below. Figure 1 shows the indexed XRD patterns
edly with deionized water and ethanol, and dried at 110 °C for for the product obtained by the hydrothermal reduction of
24 h. In analogous reactions, 2-propanol was substituted with
the precursor with 2 mL of 2-propanol for 7 days. The
methanol, ethanol, and octanol.
Characterization. Powder X-ray diffraction (XRD) data was
normalized theoretical intensities match very well with the
collected in Bragg-Brentano geometry using a Rigaku Ultima IV experimental diffraction pattern. A visualization of the crystal
structure depicting the CuxV2O5 unit cell is shown in Figure
(26) Ma, H.; Zhang, S.; Ji, W.; Tao, Z.; Chen, J. J. Am. Chem. Soc. 2008, 2. As noted above, two distinct locations inside the V2O5
130 (15), 5361–5367.
(27) Melghit, K.; Al-belushi, M. Mater. Lett. 2008, 62 (19), 3358–3360. framework are partially occupied by Cu+ ions. The Cu+ ions
(28) Liu, Y.; Zhang, Y.; Zhang, M.; Qian, Y. J. Cryst. Growth 2006, 289 are located on the mirror plane of 4i (tetrahedrally coordi-
(29) Xiong, C. R.; Aliev, A. E.; Gnade, B.; Balkus, K. J. ACS Nano 2008, nated by four oxygen atoms) and on the 8j position
2 (2), 293–301.
(30) Prokoﬁev, A. V.; Kremer, R. K.; Assmus, W. J. Cryst. Growth 2001, (32) Galy, J.; Lavaud, D.; Casalot, A.; Hagenmuller, P. J. Solid State Chem.
231 (4), 498–505. 1970, 2 (4), 531–543.
(31) Sakurai, Y.; Ohtsuka, H.; Yamaki, J.-i. J. Electrochem. Soc. 1988, (33) Savariault, J. M.; Deramond, E.; Galy, J. Z. Kristallogr. 1994, 209
135 (1), 32–36. (5), 405–412.
Inorganic Chemistry, Vol. 48, No. 7, 2009 3147
Patridge et al.
Figure 1. XRD pattern of CuxV2O5 nanowires prepared by the hydrothermal
reduction of CuV2O6 by 2-propanol for 7 days shown alongside the PDF
pattern 97-007-7609 corresponding to the diffraction pattern of Cu0.59V2O5.
Figure 3. XRD patterns of CuxV2O5 nanowires prepared by the reduction
of micrometer-size bulk CuV2O6 by (A) 2 mL, (B) 500 µL, (C) 250 µL,
(D) 100 µL of 2-propanol. (E) XRD pattern of micrometer-sized CuV2O6.
phase with the nominal stoichiometry Cu3(OH)2V2O7 · 2H2O
(97-007-3282) is noted and the relative concentration of this
phase appears to be signiﬁcantly greater when the 2-propanol
content is decreased in the reaction mixture. This hydrated
phase has been proposed as an intermediate to the formation
of CuV2O6 nanowires by a hydration, exfoliation, splitting
process and is a naturally occurring mineral found in oxidized
zones of vanadium-containing hydrothermal deposits.34 The
degree of hydration appears to vary somewhat across
different experimental runs as indicated by DSC measure-
Figure 2. Crystal Structure of Cu(0.55 - 0.65)V2O5. Cu (blue) atoms reside at
ments. However, XRD measurements indicate the retention
two positions within the V2O5 framework (red VO6 and green VO5). The of the basic volborthite framework. As discussed in more
unit cell is visible near the middle of the image looking down the b-axis. detail below, this phase is likely a byproduct of the
disproportionation reaction that yields CuxV2O5 nanowires.
(trigonally coordinated by three oxygen atoms). In this Most notably, these copper vanadium bronze nanowires are
structure, two crystallographically distinct vanadium atoms, not formed when CuV2O6 is treated hydrothermally with DI
V1 and V2, form double VO6 octahedra with edge sharing water without the addition of any alcohols.
along the b-direction. The third distinct, vanadium site, V3, Upon hydrothermal treatment in the presence of alcohols,
connects the double octahedra along the c-direction and has a disproportionation reaction is thought to yield the Cu-rich
an edge-sharing square pyramidal local geometry. Because volborthite phase and the copper-deﬁcient CuxV2O5 phase
of variable copper content, convergent beam electron dif- as per
fraction at low temperature has been used to establish the
2CuV2O6+3RCH2OH f 0.33Cu3(OH)2V2O7·2H2O +
C2/m space group assignment for these ′ vanadium
bronzes.13 Figures 1 and 3 show noticeable differences in 1.66Cu0.60V2O5 + 3RCHO (1)
the relative intensities of reﬂections for samples prepared
by hydrothermal reduction with different alcohols for varying Notably, some deviation from the above stoichiometries
times. These changes can be attributed to the strongly is likely, especially with regards to the extent of hydration
preferred orientation present in the 1D nanowire products and hydroxylation of the volborthite phase but is difﬁcult to
that is somewhat retained even after mechanical grinding of monitor because of the low concentrations of this phase. The
the samples (which does not appear to break the nanowires). stoichiometry of this reaction implies the predominance of
Figure 3 compares the XRD pattern of the CuV2O6 starting the copper-deﬁcient vanadium bronze phase, as is indeed
material to the products obtained after hydrothermal reduc- experimentally observed. However, the relative proportion
tion with varying amounts of 2-propanol. A very low of the Cu0.60V2O5 nanowires in the product seems to be in
intensity peak at 29.6° which matches well with the strongest excess of the amounts expected from eq 1. This can be
reﬂection of the precursor CuV2O6 phase is seen for all the attributed to the hydrothermal decomposition of the volbor-
products evidencing the persistence of some of the starting (34) Zhang, S.; Li, W.; Li, C.; Chen, J. J. Phys. Chem. B 2006, 110 (49),
material. Most notably, the presence of a hydrated volborthite 24855–24863.
3148 Inorganic Chemistry, Vol. 48, No. 7, 2009
Single-Crystalline CuxV2O5 Nanowires
thite phase into CuV2O6 and CuO as reported previously in
Cu3(OH)2V2O7·2H2O f CuV2O6+2CuO + 3H2O (2)
This reaction yields CuV2O6, which is then further
transformed to the copper vanadium bronze nanowires
according to eq 1. XPS measurements indicate the presence
of some Cu(II) species corresponding to trace CuO present
in the samples; some soluble copper species are also likely
lost during the ﬁltration of the nanowire product.
At low alcohol concentrations (100-500 µL), the trans-
formation of CuV2O6 to CuxV2O5 is incomplete even after
reaction for 7 days. The CuxV2O5 peak increases in intensity
as the 2-propanol concentration crosses a certain threshold
for the transformation and CuxV2O5 becomes the dominant
phase. The origin of this strong concentration dependence Figure 4. (A) SEM images of CuxV2O5 nanowires showing the high yield
is likely the heterogeneous nature of the reaction, which is of synthesis (top-left), a few single shorter nanowires spin-coated onto a
Si/SiO2 substrate (bottom-left), (B) HRTEM image of two wires, overlapped
expected to be diffusion limited and requires the intercalation and aligned, with corresponding (C) showing a lattice-resolved image and
of the reducing agent between the CuV2O6 layers. The extent (D) indexed SAED pattern of the lattice area.
of alcohol intercalation within the layered frameworks is
expected to depend on the alcohol concentration, since the
intimate contact of the reactants can only occur upon the
intercalation of the alcohol molecules within the CuV2O6
Notably, the heterogeneous dehydrogenation of alcohols
is known to be catalyzed by copper, and indeed forms the
basis for a process to synthesize acetone at elevated tem-
peratures (300 °C),35-38 conditions not very far removed
from those achieved during hydrothermal treatment. Other
alcohols (methanol, ethanol, octanol) are analogously able
to act as reducing agents as indicated in eq 1, being oxidized Figure 5. SEM images of CuxV2O5 nanowires prepared by the reduction
to their corresponding aldehydes, ketones, or carboxylic acids of CuV2O6 by (A) 250 µL 2-propanol, (B) 2 mL octanol.
in the process.
SEM and TEM images indicate the formation of single-
crystalline high-aspect-ratio nanowires of CuxV2O5 upon the
hydrothermal reduction of CuV2O6 by aliphatic alcohols. The
nanowires present a smooth surface and have uniform
diameters along the length that are typically <100 nm, as
shown in Figure 4. There is no noticeable tapering even in
extremely long nanowires. The HRTEM image in Figure 4C
illustrates the single-crystalline nature of the nanowires. The Figure 6. Intermediates observed during the nanowire formation process.
lattice spacing of 0.731 nm matches well with the separation The presence of lamellar structures that are splitting into nanowires is clearly
between (2 0 0) crystal planes running parallel to the long
axis of the nanowire. The single-crystalline nature of these
of CuV2O6 by different alcohols as per eq (1). Upon reaction
nanowires is in marked contrast to the high concentration
for 7 days, methanol, ethanol, 2-propanol, and 1-octanol all
of grain boundaries found in CuV2O6 nanowires reported
yield high-aspect-ratio nanowire geometries, likely being
previously in the literature.23 The indexed SAED inset to
themselves oxidized in the process to aldehydes and ketones
Figure 4B shows the corresponding planes in the pattern.
or the corresponding carboxylic acids as V5+ is reduced to
The SEM images in Figures 5 and 6 provide further insight
into the growth mechanism. Figure 5 shows SEM images of V4+ along the V2 ladder and Cu2+ is reduced to Cu+. We
CuxV2O5 nanowires obtained by the hydrothermal reduction have found no evidence for the formation of volborthite
nanowires or the presence of volborthite segments in single-
(35) Chanda, M.; Mukherjee, A. K. Ind. Eng. Chem. Res. 1987, 26 (12), crystalline CuxV2O5 nanowires (vide infra) indicating that
2430–2437. the minor phase stays as micrometer-sized particles separable
(36) Katona, T.; Molnar, A.; Bartok, M. Mater. Sci. Eng, A 1994, 182,
1095–1098. from the nanowires by a gentle centrifugation step. The
(37) Marchi, A. J.; Fierro, J. L. G.; Santamaria, J.; Monzon, A. Appl. Catal. nuclei of the predominant phase, layered CuxV2O5, are ﬁrst
1996, 142 (2), 375–386.
(38) Molnar, A.; Varga, M.; Mulas, G.; Mohai, M.; Bertoti, I.; Lovas, A.;
´ formed by the disproportionation reaction shown in eq 1.
Cocco, G. Mater. Sci. Eng., A 2001, 304-306, 1078–1082. The intercalation/reduction of CuV2O6 by the alcohol
Inorganic Chemistry, Vol. 48, No. 7, 2009 3149
Patridge et al.
Figure 8. Current vs voltage plot measured for a pressed pellet of CuxV2O5
using the four-point probe technique; least-squares regression ﬁt (red) and
data points (black).
ires obtained from the hydrothermal reduction of CuV2O6
by 2-propanol for 7 days. XPS data has also been acquired
for bulk V2O5 and clearly indicates the V5+ oxidation state
of the orthorhombic framework. For the nanowire samples,
the V2p3/2 peak appears at 517.5 eV and the V2p1/2 is at
524.5 eV, yielding a spin-orbit splitting of 7.00 eV.
The O1s region of CuxV2O5 shows multiple peaks evidenc-
ing the several crystallographically distinct oxygen sites and
different bonding environments in the CuxV2O5 nanowire
samples. At least two distinct curves at 529.3 and 531.6 eV
can be ﬁtted to the O1s spectra. The V2p3/2 and V2p1/2 region
also show broadening, peak multiplicity, and a decrease in
the peak energies owning to the reduction of V5+ to V4+
(and perhaps even some V3+) at 515.3 and 523.8 eV. As
noted above, charge disproportionation on the V2 ladder is
thought to be the primary origin of the conductivity of these
nanowires. The V4+ ions observed here likely reside on this
V2 ladder and are formed by the reduction of V5+ sites in
the CuV2O6 network during hydrothermal reduction with
aliphatic alcohols. Cu2+ in CuV2O6 is also reduced during
Figure 7. XPS spectra for CuxV2O5 nanowires (A) Copper 2p, (B) Oxygen
1s, (C) Vanadium 2p. the hydrothermal reduction process, and the electrons from
the Cu ions occupying interstitial sites may serve to reduce
molecules results in the exfoliation of micrometer-sized V5+ to V4+ on the V2 ladder. The Cu2p3/2 region shows
CuV2O6 particles, yielding thin lamellar morphologies. Figure distinctive signals corresponding to Cu2+ and Cu+ at 934.6
6 provides clear evidence for the formation of such lamellar and 932.4 eV, respectively. Part of the Cu2+ signal likely
intermediates. This ﬁgure also shows nanowires being split originates from the CuV2O6 precursor and volborthite and
from the nanosheet intermediates. The splitting of the reduced CuO byproduct noted above. However, it is also possible
lamellar intermediates yields CuxV2O5 nanowires as water for Cu2+ to occupy some of the interstitial sites within the
and alcohol molecules are deintercalated from the layered CuxV2O5 bronzes. Savariault et al. have noted the occupation
structure. Similar ripening-exfoliation-splitting mechanisms of tunnel sites by both Cu+ and Cu2+ in micrometer-sized
have been implicated in the formation of 1D nanostructures CuxV2O5.33
from other layered precursors. In AgVO3, V2O5, and TiO2, Electrical transport measurements support the metallic
the stresses generated within exfoliated nanosheets are nature of the synthesized wires. Figure 8 shows the
relieved by disintegration into nanowire fragments. In the current-voltage plots measured for pellets of CuxV2O5
reactions reported here, an additional driving force likely nanowires by the four-point probe method to eliminate the
comes from the placement of copper in more energetically effects of contact resistance. The linear relationship of the
favorable sites in the ′-CuxV2O5 bronzes. current-voltage curve and the relatively low sheet resistance
XPS has been used to further structurally characterize the of 2.7 kΩ suggests the metallic nature of the nanowires (the
obtained CuxV2O5 nanowires. Figure 7 shows O 1s, V 2p, resistance is <200 times that of a V2O5 pellet). Notably, in
and Cu 2p high-resolution XPS spectra acquired for nanow- a pressed pellet measurement, hopping between wires likely
3150 Inorganic Chemistry, Vol. 48, No. 7, 2009
Single-Crystalline CuxV2O5 Nanowires
Figure 9. CuxV2O5 (red) infrared absorption is markedly less intense in
comparison to the CuV2O6 precursor and the empty V2O5 framework,
evidencing the high carrier density in these nanowires. The plotted spectra
have been offset for clarity. Figure 10. Normalized NEXAFS data for V2O5, CuV2O6, and CuxV2O5
nanowires. The inset shows a magniﬁed view of the O K edge region.
dominates transport but the low resistance values nevertheless whereas the O K-edge spectra represent the p-projected
evidence the high conductivity of these nanowires. unoccupied density of states of the valence levels. The strong
Fourier transform infrared (FTIR) spectra provide further hybridization of the O 2p levels with the V-3d levels enables
insight into the electronic structure of the obtained CuxV2O5 the observation of transitions into these unoccupied levels
bronzes (Figure 9). The V2O5 tunnel framework has char- as distinct features in the O K-edge NEXAFS spectra.
acteristic IR peaks at 1010, 825, and 500-600 cm-1 that The NEXAFS data in Figure 10 shows V L-edge and O
can be attributed to V)O stretching (from the vanadyl K-edge regions for V2O5, the CuV2O6 precursor and the ′-
oxygen), V-O-V coupled stretching, and V-O-V sym- CuxV2O5 vanadium bronze nanowires. The two broad peaks
metric stretching modes respectively.39 The precursor main- centered at ∼518 and 525 eV are the V L3 and L2 peaks
tains the absorption characteristics of V2O5 at 830 and 550 arising from V2p3/2fV3d and V2p1/2fV3d transitions,
cm-1 but shows a new absorption peak at ∼ 930 cm-1, which respectively. The spin-orbit splitting between the V L3 and
is in agreement with Baran and Cabello’s study of CuV2O6 L2 peaks is 7.0 eV for V2O5, 6.6 eV for CuV2O6, and 6.5 eV
and the inﬂuence of copper in reducing the energy differences for the CuxV2O5 nanowires. Havecker et al. have shown that
between the various V-O bending frequencies.40 Remark- the positions and lineshapes of V L3 peaks depend sensitively
ably, the IR absorption is very signiﬁcantly attenuated in on both the vanadium formal valence and the local coordina-
the obtained CuxV2O5 nanowires. This is consistent with tion environment as measured by the bond length.42 The
previous literature results on metallic copper vanadium CuV2O6 sample shows a splitting of the V L3 peak that
bronzes and can be attributed to the high carrier concentra- undoubtedly arises from differences in bond lengths arising
tions in these metallic nanowires, which strongly suppresses from the crystallographically inequivalent V sites in the
infrared absorption.41 Very similar IR spectra have been triclinic crystal structure since the formal valence of all the V
obtained for hydrothermally synthesized nanowires prepared sites is V5+ in this structure. The V L3 peak for the CuxV2O5
using different aliphatic alcohols corroborating the strong is more similar to the V2O5 data than the spectra for the bulk
driving force for the stabilization of the CuxV2O5 bronzes CuV2O6 precursor. Ma et al. have calculated the V 3d
upon the reduction of CuV2O6. projected density of states for the three crystallographically
Further characterization of the electronic structure of the distinct V sites in vanadium bronzes and have shown that
obtained CuxV2O5 nanowires comes from soft X-ray absorp- differences in the unoccupied density of states for the three
tion spectroscopy measurements (Figure 10). NEXAFS is a types of atoms are very marginal and not enough to explain
powerful element-speciﬁc tool for probing the frontier orbital the observed splitting of the V L3 peak noted in measure-
states of CuxV2O5 based on the excitation of core hole states ments of bulk vanadium bronze samples.15a A broadening
to partially ﬁlled and empty states. Given the selection rules and distinct splitting has also been observed for the vanadium
for NEXAFS, ∆l ) (1, the V L-edge NEXAFS spectra bronze nanowire samples measured here and in analogy to
represent the d-projected unoccupied density of states, measurements of bulk samples can be attributed to the
presence of mixed valence vanadium ions, providing strong
(39) Mori, K.; Miyamoto, A.; Murakami, Y. J. Chem. Soc., Faraday Trans.
1987, 1 (83), 3303. evidence for charge disproportionation in these structures.
(40) Baran, E. J.; Cabello, C. I.; Nord, A. G. J. Raman Spectrosc. 1987,
18 (6), 405–407. ¨
(42) Havecker, M.; Knop-Gericke, A.; Mayer, R. W.; Fait, M.; Bluhm,
(41) Robb, F. Y.; Glaunsinger, W. S. J. Solid State Chem. 1979, 30 (1), ¨
H.; Schlogl, R. J. Electron Spectrosc. Relat. Phenom. 2002, 125 (2),
Inorganic Chemistry, Vol. 48, No. 7, 2009 3151
Patridge et al.
Most notably, the difference in the splitting of the L3 peak O K-edge peaks result from unique two- and three-
(energy difference ∆1 of 1.95 eV) and the splitting of the coordinated oxygen atoms in V2O5. CuxV2O5 is similar to
O-K-edge peak (energy difference ∆2 ) 2.4 eV) establishes V2O5 with clear splitting of the t2g* and eg* peaks. The
charge disproportionation and not crystallographically in- lineshapes of the O K-edge spectra for CuxV2O5 are remark-
equivalent sites as the origin of the peak multiplicity. ably similar which is not surprising given the extent to which
Notably, some contribution to the changes in peak position the V2O5 framework is retained upon the intercalation of
likely arise from the distortion of the VO6 octahedron to a copper ions. The peak broadening can be attributed to the
VO5 polyhedron and one very weak V-O bond upon the presence of a greater number of crystallographically in-
introduction of copper, which causes a small increase in equivalent oxygens (8 opposed to 3 in V2O5). The crystal-
orbital overlap thus raising the energies of the antibonding lographically distinct oxygen atoms are expected to be
orbitals. Notably, the low-energy 515 eV peak corresponding slightly different in the overlapping O2p-V3d hybridization
to transitions into V 3dxy levels hybridized with 2px/2py and thus antibonding energies. The levels may also be
orbitals on the edge-sharing oxygens in V2O5 are lost in the somewhat hybridized with Cu 3d orbitals further modifying
CuxV2O5 nanowires.43,44 This split-off conduction band peak the unoccupied density of states in CuxV2O5 nanowires.15a
is thought to be responsible for the n-type semiconducting The weakly structured peaks above 535 eV arise from
nature of V2O5 that is no longer retained in CuxV2O5 transitions from O1s to O2p levels hybridized with V4s and
nanowires.43,44 The V L2 peak is broadened by the V4p states. The signiﬁcant spectral weight in this region
Coster-Kronig Auger decay process into a 2p3/2 hole that further corroborates the strong covalent contributions to
does not exist for the L3 excitation and is less useful for bonding in this structure.45
understanding the electronic structure of the nanowires In conclusion, single-crystalline copper vanadium bronze
although the splitting of peaks noted above is indeed nanowires CuxV2O5 have been synthesized via a simple
discernible even for this spectral feature. hydrothermal approach based on the reduction of a solid-
The O K-edge spectra of the nanowires can be explained state CuV2O6 precursor by small-molecule aliphatic alcohols.
with reference to the data for bulk V2O5. The strong Electron microscopy observations show the formation of
hybridization of O 2p states with V 3d states leads to the clean and uniform wires with aspect ratios exceeding 300.
observation of transitions into these orbitals. The splitting XPS, FTIR, transport, and NEXAFS data evidence charge
of the O K-edge spectra into distinct features arises from disproportionation and high carrier densities in the CuxV2O5
the crystal ﬁeld splitting of the V 3dz2 and 3dx2-y2 eg* levels nanowires even at room temperature. The availability of these
from V 3dxy, 3dyz, and 3dxz t2g* levels as a result of the clean nanowire samples will allow investigation of the
roughly cubic ﬁeld.43,44 The intensity of the two peaks inﬂuence of ﬁnite size on the remarkable electronic and
relative to the V L-edge resonances arises from the consider- electrochemical properties of vanadium bronzes. These high-
able covalency of the V-O bonds, as is typical of early aspect-ratio copper vanadium bronzes are especially of
transition metal oxides.45 The V2O5 experimental data are interest as building blocks for novel cathode architectures
consistent with previous literature results and spectra pre- showing enhanced Li-ion diffusion kinetics and as highly
dicted from calculated V3d and O2p-projected unoccupied conducting (and potentially superconducting) elements of
density of states.43,44,46,47 The peak at 529.5 represents the nanoscale devices. Future work will focus on transport
O1s transition to 2px-3d and 2py-3d overlap orbitals in VO6 measurements of individual nanowires to map out the
octahedra. The higher energy peak arises from better overlap inﬂuence of the nanowire dimensions on the quantum phase
between 2pz and 3dz2 and 3dx2-y2 creating high energy slips below the critical temperature.
antibonding orbitals for the singly coordinated apical double
Acknowledgment. S.B. acknowledges startup funding
bond oxygen O(1) in V2O5.15a,43 Other contributions to the
from the University at Buffalo for support of this work. We
gratefully acknowledge Dr. Peter Bush and Dr. Yueling Qin
(43) Eyert, V.; Hock, K. H. Phys. ReV. B 1998, 57, 12727–12737.
(44) Goering, E.; Muller, O.; Klemm, M.; denBoer, M. L.; Horn, S. Philos. for help with SEM and HRTEM measurements. Certain
Mag. B 1997, 75 (2), 229–236. commercial names are presented in this manuscript for
(45) de Groot, F. M. F.; Grioni, M.; Fuggle, J. C.; Ghijsen, J.; Sawatzky,
G. A.; Petersen, H. Phys. ReV. B 1989, 40 (8), 5715. purposes of illustration and do not constitute an endorsement
(46) Willinger, M.; Pinna, N.; Su, D. S.; Schloegl, R. Phys. ReV. B 2004, by the National Institute of Standards and Technology.
69 (15), 155114/1–155114/7.
(47) Kolczewski, C.; Hermann, K. Phys. Scr. 2005, T115, 128–130. IC802408C
3152 Inorganic Chemistry, Vol. 48, No. 7, 2009